ME 350 – Lecture 9 – Chapter 11. METAL CASTING PROCESSES Sand Casting Other Expendable Mold Casting Processes Permanent Mold Casting Processes Casting Quality Product Design Considerations. Making the Sand Mold.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
METAL CASTING PROCESSES
Pattern – a model of the part, slightly enlarged to account for shrinkage and machining allowances
Types of patterns used in sand casting:
(a) solid pattern, (b) split pattern, (c) match‑plate pattern
(d) cope and drag pattern
Full‑scale model of interior surfaces of part
(a) Core held in place in the mold cavity by chaplets, (b) possible chaplet design, (c) casting with internal cavity.
Fb = Wm ‑ Wc
where Fb = buoyancy force; Wm = weight of molten metal displaced; and Wc = weight of core
Silica (SiO2) or silica mixed with other minerals
Casting process in which the mold is a thin shell of sand held together by thermosetting resin binder
Steps in shell‑molding: (1) a match‑plate or cope‑and‑drag metal pattern is heated and placed over a box containing sand mixed with thermosetting resin.
Steps in shell‑molding: (2) box is inverted so that sand and resin fall onto the hot pattern, causing a layer of the mixture to partially cure on the surface to form a hard shell; (3) box is repositioned so that loose uncured particles drop away;
Steps in shell‑molding: (4) sand shell is heated in oven for several minutes to complete curing; (5) shell mold is stripped from the pattern;
Steps in shell‑molding: (6) two halves of the shell mold are assembled, supported by sand or metal shot in a box, and pouring is accomplished; (7) the finished casting with sprue removed.
Uses a mold of sand packed around a polystyrene foam pattern which vaporizes when molten metal is poured into mold
Expanded polystyrene casting process: (1) pattern of polystyrene is coated with refractory compound;
Expanded polystyrene casting process: (2) foam pattern is placed in mold box, and sand is compacted around the pattern;
Expanded polystyrene casting process: (3) molten metal is poured into the portion of the pattern that forms the pouring cup and sprue. As the metal enters the mold, the polystyrene foam is vaporized ahead of the advancing liquid, thus the resulting mold cavity is filled.
A pattern made of wax is coated with a refractory material to make mold, after which wax is melted away prior to pouring molten metal
Steps in investment casting: (1) wax patterns are produced, (2) several patterns are attached to a sprue to form a pattern tree
Steps in investment casting: (3) the pattern tree is coated with a thin layer of refractory material, (4) the full mold is formed by covering the coated tree with sufficient refractory material to make it rigid
Steps in investment casting: (5) the mold is held in an inverted position and heated to melt the wax and permit it to drip out of the cavity, (6) the mold is preheated to a high temperature, the molten metal is poured, and it solidifies
Steps in investment casting: (7) the mold is broken away from the finished casting and the parts are separated from the sprue
A one‑piece compressor stator with 108 separate airfoils made by investment casting (photo courtesy of Howmet Corp.).
Mold metal must have higher melt temperature than casting metal
Steps in permanent mold casting: (1) mold is preheated and coated
Steps in permanent mold casting: (2) cores (if used) are inserted and mold is closed, (3) molten metal is poured into the mold, where it solidifies.
A permanent mold casting process in which molten metal is injected into mold cavity under high pressure
A family of casting processes in which the mold is rotated at high speed so centrifugal force distributes molten metal to outer regions of die cavity. Example:
Misrun – metal solidified before completely filling cavity. Cold shut – metal has flowed together but failed to fuse or blend into a solid mass.
Increase pour temperature, increase sand permittivity, or increase height of downsprue
Metal splatters during pouring and solid globules form and become entrapped in casting
Increase diameter of pouring cup or slow down pour
Depression in surface or internal void caused by solidification shrinkage that restricts amount of molten metal available in last region to freeze
Increase riser volume to surface area ratio
Balloon‑shaped gas cavity or many small gas cavities just below the surface
Decrease pour temperature or increase sand permittivity
When fluidity of liquid metal is high, it may penetrate into sand mold or core, causing casting surface to consist of a mixture of sand grains and metal
Lower pour temperature or decrease sand permittivity
Design change to eliminate the need for using a core: (a) original design, and (b) redesign.